Abstract
Through intense research on Weyl semimetals during the past few years, we have come to appreciate that typical Weyl semimetals host many Weyl points. Nonetheless, the minimum nonzero number of Weyl points allowed in a timereversal invariant Weyl semimetal is four. Realizing such a system is of fundamental interest and may simplify transport experiments. Recently, it was predicted that TaIrTe_{4} realizes a minimal Weyl semimetal. However, the Weyl points and Fermi arcs live entirely above the Fermi level, making them inaccessible to conventional angleresolved photoemission spectroscopy (ARPES). Here, we use pumpprobe ARPES to directly access the band structure above the Fermi level in TaIrTe_{4}. We observe signatures of Weyl points and topological Fermi arcs. Combined with ab initio calculation, our results show that TaIrTe_{4} is a Weyl semimetal with the minimum number of four Weyl points. Our work provides a simpler platform for accessing exotic transport phenomena arising in Weyl semimetals.
Introduction
A Weyl semimetal is a crystal which hosts emergent Weyl fermions as electronic quasiparticles. In an electronic band structure, these Weyl fermions correspond to accidental degeneracies, or Weyl points, between two bands^{1,2,3,4,5}. It is wellunderstood that Weyl points can only arise if a material breaks either spatial inversion symmetry, \({\cal I}\), or timereversal symmetry, \({\cal T}\) ^{6,7,8,9}. At the same time, in a Weyl semimetal, symmetries of the system tend to produce copies of Weyl points in the Brillouin zone. As a result, typical Weyl semimetals host a proliferation of Weyl points. For instance, the first Weyl semimetals observed in experiment, TaAs and its isoelectronic cousins, have an \({\cal I}\) breaking crystal structure, which gives rise to a band structure hosting 24 Weyl points distributed throughout the bulk Brillouin zone^{10,11,12,13,14,15,16,17}. However, most of these Weyl points can be related to one another by the remaining symmetries of TaAs, namely two mirror symmetries, C _{4} rotation symmetry and \({\cal T}\). In the Mo_{ x }W_{1−x }Te_{2} series, which has recently been under intensive theoretical and experimental study as a Weyl semimetal with strongly Lorentzviolating, or Type II, Weyl fermions, mirror symmetry and \({\cal T}\) relate subsets of the eight Weyl points^{18,19,20,21,22,23,24,25}. As another example, according to calculation, the Weyl semimetal candidate SrSi_{2} hosts no fewer than 108 Weyl points, copied in sets of 18 by three C _{4} rotation symmetries^{26}. However, as we review below, it is wellknown that the minimal nonzero number of Weyl points allowed is 4 for a \({\cal T}\) invariant Weyl semimetal. Realizing such a minimal Weyl semimetal is not only of fundamental interest, but is also practically important, because a system with fewer Weyl points may exhibit simpler properties in transport and be more suitable for device applications.
Recently, TaIrTe_{4} was predicted to be a Weyl semimetal with only four Weyl points^{27}. It was further noted that the Weyl points are associated with Type II Weyl fermions, providing only the second example of a Type II Weyl semimetal after the Mo_{ x }W_{1−x }Te_{2} series^{18}. Moreover, the Weyl points are wellseparated in momentum space, with substantially larger topological Fermi arcs as a fraction of the size of the surface Brillouin zone than other known Weyl semimetals. Lastly, TaIrTe_{4} has a layered crystal structure, which may make it easier to carry out transport experiments and develop device applications. All of these desirable properties have motivated considerable research interest in TaIrTe_{4}. At the same time, one crucial challenge is that the Weyl points and topological Fermi arcs are predicted to live entirely above the Fermi level in TaIrTe_{4}, so that they are inaccessible to conventional angleresolved photoemission spectroscopy (ARPES).
Here, we observe signatures of Weyl points and topological Fermi arcs in TaIrTe_{4}, realizing the first minimal \({\cal T}\) invariant Weyl semimetal. We first briefly reiterate a wellknown theoretical argument that the minimum number of Weyl points for a \({\cal T}\) invariant Weyl semimetal is four. Then, we present ab initio calculations showing a nearly ideal configuration of Weyl points and Fermi arcs in TaIrTe_{4}. Next, we use pumpprobe ARPES to directly access the band structure of TaIrTe_{4} above the Fermi level in experiment. We report the observation of signatures of Weyl points and topological Fermi arcs. Combined with ab initio calculations, our results demonstrate that TaIrTe_{4} has four Weyl points. We conclude that TaIrTe_{4} can be viewed as a minimal Weyl semimetal, with the simplest configuration of Weyl points allowed in a \({\cal T}\) invariant crystal.
Results
Minimum number of Weyl points under timereversal symmetry
We first reiterate wellknown arguments that four is the minimum number of Weyl points allowed in a \({\cal T}\) invariant Weyl semimetal. A Weyl point is associated with a chiral charge, directly related to the chirality of the associated emergent Weyl fermion. It can be shown that for any given band the sum of all chiral charges in the Brillouin zone is zero. Further, under \({\cal T}\) a Weyl point of a given chiral charge at k is mapped to another Weyl point of the same chiral charge at −k. This operation of \({\cal T}\) on a chiral charge is illustrated in Fig. 1a on the blue Weyl points with +1 chiral charge (the same arrow applies for the red Weyl points but is not drawn explicitly). Now, if an \({\cal I}\) breaking Weyl semimetal has no additional symmetries which produce copies of Weyl points, then the minimum number of Weyl points is fixed by \({\cal T}\) symmetry and the requirement that total chiral charge vanish. In the simplest case, \({\cal T}\) will produce two copies of Weyl points of chiral charge +1, as shown in Fig. 1a. To balance these out, the system must have two chiral charges of −1, also related by \({\cal T}\). In this way, the minimum number of Weyl points in a \({\cal T}\) invariant Weyl semimetal is four. This simple scenario is realized in TaIrTe_{4}. The crystal structure of TaIrTe_{4} is described by space group 31 (Pmn2_{1}), lattice constants a = 3.77 Å, b = 12.421 Å, and c = 13.184 Å, with layered crystal structure, see Fig. 1b. We note that TaIrTe_{4} takes the same space group as Mo_{ x }W_{1−x }Te_{2}, but has a unit cell doubled along b. To study where the Weyl points show up in TaIrTe_{4} we present the electronic band structure along various highsymmetry directions, see Brillouin zone and ab initio calculation in Fig. 1c, d. Enclosed by the rectangular box along Γ − S is a crossing region between the bulk conduction and valence bands that gives rise to Weyl points. A more detailed calculation shows that the Weyl points have tilted over, or Type II, Weyl cones and that they live above the Fermi level, E _{F} at k _{ z } = 0^{27}. A cartoon schematic of the resulting constant energy contour at the energy of the Weyl points, E _{B} = E _{W}, is shown in Fig. 1e. The electron and hole pockets form Type II Weyl cones where they touch (red and blue marks). In this way, TaIrTe_{4} has four Weyl points, the minimal number allowed in an \({\cal I}\) breaking Weyl semimetal. The overall electronic structure of TaIrTe_{4} near E _{F} is similar to Mo_{ x }W_{1−x }Te_{2}, but we note that the role of the electron and hole pockets is reversed in TaIrTe_{4} relative to Mo_{ x }W_{1−x }Te_{2}. Also, Mo_{ x }W_{1−x }Te_{2} has eight Weyl points, so it is not minimal, and we will see that TaIrTe_{4} also hosts larger Fermi arc surface states than Mo_{ x }W_{1−x }Te_{2}. To study the expected Fermi arcs in TaIrTe_{4}, we present an energydispersion cut along a pair of projected Weyl points along k _{ y }, Fig. 1f. We clearly observe a large single Fermi arc surface state at ~0.1 eV above the Fermi level that is ~0.25 Å^{−1} long and connecting a pair of ±1 chiral charged Weyl points along k _{ y }. In this way, TaIrTe_{4} provides a minimal Weyl semimetal with large Fermi arcs. Like the Weyl points, the Fermi arcs live well above the Fermi level, making them inaccessible to conventional ARPES.
Unoccupied band structure of TaIrTe_{4} by pumpprobe ARPES
Next, we use pumpprobe ARPES to directly access the unoccupied band structure of TaIrTe_{4} up to E _{B} > 0.2 eV and we find excellent agreement with calculation. In our experiment, we use a 1.48 eV pump laser pulse to excite electrons into lowlying states above the Fermi level, followed by a 5.92 eV probe laser pulse to perform photoemission^{28}. We study E _{B}−k _{ x } cuts near \(\bar \Gamma\), Fig. 2a–c, with key features marked by guides to the eye in Fig. 2d. Above the Fermi level, we see a crossinglike feature near E _{B} ~ 0.15 eV, labeled 1, and two electronlike bands, 2 and 3, extending out above E _{F}. Below the Fermi level, we observe a general holelike structure consisting of three bands, labeled 4–6. As we shift k _{ y } off \(\bar \Gamma\), we find little change in the spectrum, suggesting that the band structure is rather flat along k _{ y } near \(\bar \Gamma\). However, we can observe that band 4 moves downward in energy and becomes more intense with increasing k _{ y }. We find an excellent match between our ARPES data and ab initio calculation, Fig. 2e–g. Specifically, we identify the same crossinglike feature (green arrow) and top of band 4 (orange arrow). We can also track band 4 in k _{ y } in calculation and we find that the band moves down and becomes brighter as k _{ y } increases, in excellent agreement with the data. The electronlike structure of bands 2 and 3 and the holelike structure of bands 5 and 6 are also both captured well by the calculation. Crucially, however, we notice a shift in energy between experiment and theory, showing that the sample is holedoped by ~0.05 eV. Lastly, we plot a constant energy k _{ x }−k _{ y } cut at E _{B} = E _{F}, where we see again that there is little dispersion along k _{ y } near \(\bar \Gamma\), Fig. 2h. We also indicate the locations of the E _{B}−k _{ x } cuts of Fig. 2 and the E _{B}−k _{ y } cuts of Fig. 3, to be discussed below. Our pumpprobe ARPES measurements allow us to directly measure the electronic structure above E _{F} in TaIrTe_{4} and we find excellent match with calculation.
Evidence for a Weyl semimetal in TaIrTe_{4}
Now we demonstrate that TaIrTe_{4} is a Weyl semimetal by directly studying the unoccupied band structure to pinpoint Weyl cones and topological Fermi arcs. Based on calculation, we fix k _{ x } near the expected locations of the Weyl points, k _{ x } ∼ _{ kW} = 0.2 Å^{−1} and we study E _{B}–k _{y} cuts in ARPES, see Fig. 3a–c, with key features marked by guides to the eye in Fig. 3d. We observe two cone features, labeled 1 and 2, connected by a weak, rather flat arc feature, labeled 3. We find that the cones are most pronounced at k _{ x } ~ k _{W}, but fade for larger k _{ x }. Next, we pinpoint the Fermi arc as a small peak directly on the energy distribution curve (EDC) passing through k _{ y } = 0, see the blue curve in Fig. 3e, where the dotted black line is a fit to the surrounding features. We further track the arc candidate for k _{ x } moving away from k _{W} and we find that the arc disperses slightly upwards, by about ~10 meV, see also Supplementary Fig. 1. This dispersion is consistent with a topological Fermi arc, which should connect the Weyl points and sweep upward with increasing k _{ x } ^{29}. We further pinpoint the upper Weyl cone on a momentum distribution curve (MDC) of the k _{ x } ~ k _{W} cut, Fig. 3f. We find an excellent fit of the Weyl cone peaks to Lorentzians. Using this analysis, we can quantitatively track the dispersions of the Weyl cones and Fermi arc on the k _{ x } ~ k _{W} cut, Fig. 3g and Supplementary Fig. 2. We note that for the upper Weyl cone we track the bands by Lorentzian fits on the MDC. However, for the Fermi arc and lower Weyl cone, the relatively flat dispersion requires us to track the bands in the EDCs. The EDC peak is challenging to fit, in part because the population distribution is strongly dependent on binding energy for a pumpprobe ARPES spectrum. As a result, we track the Fermi arc and lower Weyl cone through a naive quadratic fit of the band peaks, again see Fig. 3g. We find that the peak trains are nearly linear, see also Supplementary Fig. 2. Based on our pumpprobe ARPES spectra and ab initio calculations, we propose that TaIrTe_{4} hosts two pairs of Weyl points of chiral charge ±1 at k _{ x } = ±k _{W}, connected by Fermi arcs. This particular structure of two Weyl cones connected by a Fermi arc is arguably the simplest possible, Fig. 3h. We compare our results to calculation in greater detail, Fig. 3i–k. We can easily match the Weyl cones, the Fermi arc and an upper electronlike band, labeled 5 in Fig. 3d. However, we note that from calculation we expect bands 1 and 4 to attach to form a single band, while in our data they appear to be disconnected. We suggest that this discrepancy may arise because photoemission from part of the band is suppressed by low crosssection at the photon energy used in our measurement. In addition, we do not observe good agreement with the lower feature labeled 6 in our calculation, suggesting that this intensity may arise as an artifact of our measurement. At the same time, we consistently observe the broad featureless intensity below the Fermi level in both theory and experiment. Crucially, again we find a mismatch in the Fermi level. In particular, the Weyl points are expected at E _{B} ~ 0.1 eV, but we find the Weyl points at E _{B} ~ 0.07 eV. We note that this sample was grown in a different batch than the sample of Fig. 2 and a comparison with calculation suggests that the second sample is electron doped by ~30 meV, in contrast to a ~50 meV hole doping in the first sample. We propose that the difference in doping of the two samples may arise because they were grown under slightly varying conditions. Lastly, we note that the k _{ y } position of the Weyl points shows excellent agreement in theory and experiment. In summary, we observe an arc which (1) terminates at the locations of two Weyl points; (2) appears where expected in momentum space, based on calculation; and (3) disperses upward with k _{ x }, as expected from calculation. The cones (1) are gapless at a specific k _{ x } ~ k _{W}; (2) fade for larger k _{ x }; (3) appear where expected, based on calculation; (4) are connected by the arc; (5) show up in pairs only on k _{ x } ~ k _{W}, so that there are four in the entire Brillouin zone. This provides strong evidence that TaIrTe_{4} is a minimal Weyl semimetal with four Weyl points.
Discussion
We compare TaIrTe_{4} with other Weyl semimetals and consider our results in the context of general topological theory. Weyl semimetals known to date in experiment host a greater number of Weyl points than TaIrTe_{4}. In particular, the wellexplored TaAs family of Weyl semimetals hosts 24 Weyl points and Mo_{ x }W_{1−x }Te_{2} hosts eight Weyl points^{8, 30}. We plot the configuration of Weyl points for TaAs, Mo_{ x }W_{1−x }Te_{2}, and TaIrTe_{4}, where red and blue circles denote Weyl points of opposite chirality, Fig. 4a–c. It is also interesting to note that the length of the Fermi arc in TaIrTe_{4} is much longer as a fraction of the Brillouin zone than that of TaAs or Mo_{ x }W_{1−x }Te_{2}, which can be seen clearly in the projections of the Weyl points on the (001) surface of all three systems, Fig. 4d–f. We see that our discovery of a Weyl semimetal in TaIrTe_{4} provides the first example of a minimal \({\cal I}\) breaking, \({\cal T}\) invariant Weyl semimetal. One immediate application of our results is that TaIrTe_{4} in pumpprobe ARPES may provide a platform to observe the time dynamics of carrier relaxation in a Weyl semimetal. More broadly, our results suggest that TaIrTe_{4} holds promise as a simpler material platform for studying properties of Weyl semimetals in transport and applying them in devices.
Methods
Pumpprobe angleresolved photoemission spectroscopy
Pumpprobe ARPES measurements were carried out using a hemispherical electron analyzer and a modelocked Ti:Sapphire laser system that delivers 1.48 eV pump and 5.92 eV probe pulses at a repetition rate of 250 kHz^{28}. The system is stateofthe start, with a demonstrated energy resolution of 10.5 meV, the highest among any existing femtosecond pumpprobe setup to date^{31}. The time and energy resolution used in the present measurements were 300 fs and 15 meV, respectively. The spot diameters of the pump and probe lasers at the sample were 250 and 85 μm, respectively. The delay time between the pump and probe pulses was ~106 fs. Measurements were carried out at pressures <5 × 10^{−11} Torr and temperatures ~8 K.
Single crystal growth and characterization
For growth of TaIrTe_{4} single crystals, all the used elements were stored in an argonfilled glovebox with moisture and oxygen levels less than 0.1 ppm and all manipulations were carried out in the glovebox. TaIrTe_{4} single crystals were synthesized by solid state reaction with the help of Te flux. Ta powder (99.99%), Ir powder (99.999%), and a Te lump (99.999%) with an atomic ratio of Ta/Ir/Te = 1:1:12, purchased from SigmaAldrich (Singapore), were loaded in a quartz tube and then flamesealed under a vacuum of 10^{−6} Torr. The quartz tube was placed in a tube furnace, slowly heated up to 1000 °C and held for 100 h, then allowed to cool to 600 °C at a rate of 0.8 °C h^{−1}, and finally allowed to cool down to room temperature. The shiny, needleshaped TaIrTe_{4} single crystals, see Supplementary Fig. 3a, were obtained from the product and displayed a layered structure, confirmed by the optical micrograph, Supplementary Fig. 3b, and scanning electron microscope images, Supplementary Fig. 3c. The EDX spectrum displays an atomic ratio Ta:Ir:Te of 1.00:1.13(3):3.89(6), consistent with the composition of TaIrTe_{4}, Supplementary Fig. 3d.
Ab initio band structure calculations
We computed electronic structures using the projector augmented wave method^{32, 33} as implemented in the VASP^{34,35,36} package within the generalized gradient approximation^{37} schemes. Experimental lattice constants were used^{38}. A 15 × 7 × 7 MonkhorstPack kpoint mesh was used in the computations with a cutoff energy of 400 eV. The spinorbit coupling effects were included selfconsistently. To calculate the bulk and surface electronic structures, we constructed a firstprinciples tightbinding model Hamilton, where the tightbinding model matrix elements are calculated by projecting onto the Wannier orbitals^{39,40,41}, which use the VASP2WANNIER90 interface^{42}. We used Ta d, Ir d, and Te p orbitals to construct Wannier functions, without performing the procedure for maximizing localization.
Data availability
All data is available from the authors on request.
References
Weyl, H. Elektron und Gravitation. Z. Phys 56, 330–352 (1929).
Peskin, M. & Schroeder, D. An Introduction to Quantum Field Theory (Perseus Books, 1995)
Abrikosov, A. A. & Beneslavskii, S. D. Some properties of gapless semiconductors of the second kind. J. Low Temp. Phys. 5, 141–154 (1971).
Nielsen, H. B. & Ninomiya, M. The AdlerBellJackiw anomaly and Weyl fermions in a crystal. Phys. Lett. B. 130, 389–396 (1983).
Volovik, G. E. The Universe in a Helium Droplet (Clarendon Press, 2003).
Murakami, S. Phase transition between the quantum spin Hall and insulator phases in 3D: Emergence of a topological gapless phase. New J. Phys. 9, 356 (2007).
Wan, X., Turner, A. M., Vishwanath, A. & Savrasov, S. Y. Topological semimetal and Fermiarc surface states in the electronic structure of pyrochlore iridates. Phys. Rev. B 83, 205101 (2011).
Hasan, M. Z., Xu, S.Y., Belopolski, I. & Huang, S.M. Discovery of Weyl fermion semimetals and topological fermi arc states. Ann. Rev. Cond. Matt. Phys 8, 289–309 (2017).
Hosur, P. & Qi, X. Recent developments in transport phenomena in Weyl semimetals. Comp. Rend. Phys. 14, 857–870 (2013).
Xu, S.Y. et al. Discovery of a Weyl Fermion semimetal and topological Fermi arcs. Science 349, 613–617 (2015).
Lv, B. Q. et al. Experimental discovery of Weyl semimetal TaAs. Phys. Rev. X 5, 031013 (2015).
Huang, S.M. et al. A Weyl Fermion semimetal with surface Fermi arcs in the transition metal monopnictide TaAs class. Nat. Commun. 6, 7373 (2015).
Weng, H. et al. Weyl semimetal phase in noncentrosymmetric transitionmetal monophosphides. Phys. Rev. X 5, 011029 (2015).
Xu, S.Y. et al. Discovery of a Weyl fermion state with Fermi arcs in niobium arsenide. Nat. Phys. 11, 748–754 (2015).
Xu, S.Y. et al. Experimental discovery of a topological Weyl semimetal state in TaP. Sci. Adv. 1, 10 (2015).
Zheng, H. et al. Atomicscale visualization of quantum interference on a Weyl semimetal surface by scanning tunneling microscopy. ACS Nano 10, 1378 (2016).
Yang, L. X. et al. Weyl semimetal phase in the noncentrosymmetric compound TaAs. Nat. Phys. 11, 728–732 (2015).
Soluyanov, A. et al. Type II Weyl semimetals. Nature 527, 495–498 (2015).
Chang, T.R. et al. Prediction of an arctunable Weyl Fermion metallic state in Mo_{ x }W_{1−x }Te_{2}. Nat. Commun. 7, 10639 (2016).
Sun, Y. et al. Prediction of Weyl semimetal in orthorhombic MoTe_{2}. Phys. Rev. B 92, 161107 (2015).
Wang, Z. J. et al. MoTe_{2}: a typeII Weyl topological metal. Phys. Rev. Lett. 117, 056805 (2016).
Belopolski, I. et al. Fermi arc electronic structure and Chern numbers in the typeII Weyl semimetal candidate Mo_{ x }W_{1−x }Te_{2}. Phys. Rev. B 94, 085127 (2016).
Huang, L. et al. Spectroscopic evidence for type II Weyl semimetallic state in MoTe_{2}. Nat. Mat 15, 1155–1160 (2016).
Deng, K. et al. Experimental observation of topological Fermi arcs in typeII Weyl semimetal MoTe_{2}. Nat. Phys 12, 1105–1110 (2016).
Tamai, A. et al. Fermi arcs and their topological character in the candidate typeII Weyl semimetal MoTe_{2}. Phys. Rev. X 6, 031021 (2016).
Huang, S.M. et al. New type of Weyl semimetal with quadratic double Weyl fermions. PNAS 113, 1180–1185 (2015).
Koepernik, K. et al. TaIrTe_{4} a ternary typeII Weyl semimetal. Phys. Rev. B 93, 201101 (2016).
Ishida, Y. et al. Timeresolved photoemission apparatus achieving sub20meV energy resolution and high stability. Rev. Sci. Instr. 85, 123904 (2014).
Belopolski, I. et al. Criteria for directly detecting topological fermi arcs in Weyl semimetals. Phys. Rev. Lett. 116, 066802 (2016).
Hasan, M. Z., Xu, S.Y. & Bian, G. Topological insulators, topological superconductors and Weyl fermion semimetals: discoveries, perspectives and outlooks. Phys. Scrip. T164, 014001 (2015).
Ishida, Y. et al. Quasiparticles ultrafastly releasing kink bosons to form Fermi arcs in a cuprate superconductor. Sci. Rep. 6, 18747 (2016).
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953–17979 (1994).
Kresse, G. & Joubert, J. From ultrasoft pseudopotentials to the projector augmentedwave method. Phys. Rev. B 59, 1758–1775 (1999).
Kresse, G. & Hafner, J. Ab initio molecular dynamics for openshell transition metals. Phys. Rev. B 48, 13115–13118 (1993).
Kresse, G. & Furthmüller, J. Efficiency of ab initio total energy calculations for metals and semiconductors using a planewave basis set. Comput. Mater. Sci. 6, 15–50 (1996).
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio total energy calculations using a planewave basis set. Phys. Rev. B 54, 11169–11186 (1996).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).
Mar, A., Jobic, S. & Ibers, J. A. Metalmetal vs telluriumtellurium bonding in WTe_{2} and its ternary variants TaIrTe_{4} and NbIrTe_{4}. J. Am. Chem. Soc. 114, 8963–8971 (1992).
Marzari, N. & Vanderbilt, D. Maximally localized generalized Wannier functions for composite energy bands. Phys. Rev. B 56, 12847–12865 (1997).
Souza, I., Marzari, N. & Vanderbilt, D. Maximally localized Wannier functions for entangled energy bands. Phys. Rev. B 65, 035109 (2001).
Mostofi, A. A. et al. Wannier90: a tool for obtaining maximallylocalized Wannier functions. Comp. Phys. Commun 178, 685–699 (2008).
Franchini, C. et al. Maximally localized Wannier functions in LaMnO_{3} within PBE + U, hybrid functionals and partially selfconsistent GW: an efficient route to construct ab initio tightbinding parameters for e _{ g } perovskites. J. Phys. Cond. Mat 24, 235602 (2012).
Acknowledgements
I.B. thanks Daixiang Mou and Adam Kaminski for use of their conventional laser ARPES system at Ames Laboratory & Iowa State University during the preliminary phase of this project. I.B. acknowledges the support of the US National Science Foundation GRFP. The work at Princeton is supported by the US National Science Foundation, Division of Materials Research, under Grants No. NSFDMR1507585 and No. NSFDMR1006492 and by the Gordon and Betty Moore Foundation through the EPIQS program grant GBMF4547 (Hasan). Y.I. is supported by the Japan Society for the Promotion of Science, KAKENHI 26800165. This work is also financially supported by the Singapore National Research Foundation (NRF) under NRF RF Award No. NRFRF201308, MOE Tier 2 MOE2016T21131 and MOE2016T22153 (S). T.R. C. and H.T. J. are supported by the Ministry of Science and Technology, National Tsing Hua University, National Cheng Kung University, and Academia Sinica, Taiwan. T.R. C. and H.T. J. also thank the National Center for HighPerformance Computing, the Computer and Information Networking Center of National Taiwan University, and the National Center for Theoretical Sciences, Taiwan for technical support. H.L. acknowledges the Singapore NRF under Award No. NRFNRFF201303.
Author information
Affiliations
Contributions
The project was conceived by I.B. and P.Y., with guidance from M.Z.H. I.B. carried out the pumpprobe ARPES measurements with help from D.S.S. and support from Y.I. P.Y. synthesized and characterized the single crystal TaIrTe_{4} samples under the supervision of Z.L. Y.I. built the pumpprobe ARPES setup in the laboratory of S.S., with additional support from T.K. T.R.C. carried out the ab initio calculations with help from G.C. and under the supervision of H.T.J. and H.L. I.B. analyzed the data and interpreted results with help from D.S.S., T.R.C., S.S.Z., S.Y.X., H.Z., G.C., and G.B. All authors contributed to writing the manuscript.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Belopolski, I., Yu, P., Sanchez, D.S. et al. Signatures of a timereversal symmetric Weyl semimetal with only four Weyl points. Nat Commun 8, 942 (2017). https://doi.org/10.1038/s41467017009381
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467017009381
Further reading

Weyl, Dirac and highfold chiral fermions in topological quantum matter
Nature Reviews Materials (2021)

Cycling Fermi arc electrons with Weyl orbits
Nature Reviews Physics (2021)

Engineering symmetry breaking in 2D layered materials
Nature Reviews Physics (2021)

Pressureinduced superconductivity and modification of Fermi surface in typeII Weyl semimetal NbIrTe4
npj Quantum Materials (2021)

Roomtemperature nonlinear Hall effect and wireless radiofrequency rectification in Weyl semimetal TaIrTe4
Nature Nanotechnology (2021)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.